In: Biotechnology in Pulp and Paper Manufacture: Applications and Fundamental Investigations. Chapter 28 (in press).
4th International Conference on Biotechnology in the Pulp and Paper Industry, Raleigh. NC-1989 (Butterworth Publ.) 1990
IN BIOMECHANICAL PULPING *Gary F. Leatham†, Gary C. Myers†, Theodore H. Wegner†, and Robert A. Blanchette††
USDA Forest Service, Forest Products Laboratory, One Gifford Pinchot Dr., Madison, WI 53705-2398† and Plant Pathology Department, University of Minnesota, St-Paul, Minn. 55108††
Biological agents are currently being investigated as alternatives to chemicals in pulping
wood. Recently we reported that a biomechanical pulping process that uses white-rot fungi to
treat aspen chips prior to refiner mechanical pulping can increase paper strength properties. Here
we show that fungal treatments can substantially reduce the energy required forrefiner mechanical
pulping of both aspen and loblolly pine chips. Fungal species and treatment conditions affected
the amount of energy savings. Several fungi reduced the energy required for pulping by over
20%. The maximum savings with aspen or loblolly pine were 47 and 68%, respectively. Energy
consumption analyses showed that over the range of treatments tested (1) most energy was saved
during initial chip fiberization and (2) neither chip weight nor lignin loss correlated with the
amount of energy saved. Some treatments resulting in minimal chip weight loss (< 5%) saved
the most energy. With aspen, the treatments that saved the most energy did not necessarily result
in the highest paper sheet strength properties. With loblolly pine, energy was saved with several
treatments, but paper strength was not changed.
Lignin biodegradation, biotechnology, biopulping, white-rot fungi, mechanical pulps,
Cerioporiopsis subvermispora, Dichomitus squalens, Phanerochaete chrysosporim, Phlebia
brevispora, Phlebia subserialis, Phlebia tremellosa, Pholiota mutabilis, Trametes versicolor.
Mechanical pulping processes that incorporate thermal or chemical treatments, such as
thermomechanical pulping (TMP), chemirefinermechanical pulping (CRMP), and chemithermo
mechanical pulping (CTMP), are increasing in popularity (3,8,15,20). These processes require
lower capital investment and give higher pulp yield than chemical pulping, and they produce
stronger sheets than either stone ground wood (SGW) pulping or refiner mechanical pulping
(RMP) (3,8,18). The major disadvantage of mechanical pulping processes is that they require
substantial energy to fiberize the chips and subsequently refine the pulps (3,4,12,21).
* The Forest Products Laboratory is maintained in cooperation with the University of Wisconsin, Madison. This article was written and prepared by U.S. Government employees on official time, and it is therefore in the public domain and not subject to copyright.
Attempts to save energy in mechanical pulping processes with either thermal or chemical
treatments have met with little success. Energy can be saved by increasing the saturated steam
pressure in refiners, which softens lignin, but this results in a lignin-encased fiber, which
drastically reduces sheet strength (10,11,13). Chemical pretreatments of chips increase sheet
strength (3,8,22), but they can reduce pulp yield, decrease desirable sheet optical properties (light
scattering and opacity), produce dilute waste liquor streams that require treatment, and often
increase (instead of decrease) the overall energy requirement (1,4,8,9,14,22).
The disadvantages of thermal and chemical treatments have prompted interest in evaluating
the potential of biological treatments. The biopulping processes under investigation are generally
based on the concept of using lignin-degrading fungi such as
selectively remove lignin (2,5-7,16,17,19).
Recently, we obtained promising results with a nonoptimized bench-scale biomechanical
pulping process that uses white-rot basidiomycetes to treat aspen chips prior to mechanical
pulping (16). Handsheets produced from aspen chips treated in rotating drum (16) or stationary
tray bioreactors for four weeks showed substantial increases in burst, tensile, and tear strength
indexes. Maximal strength improvement was gained with less than 5% chip weight loss,
showing that the process does not require bulk removal of lignin or other major wood polymers.
Here we report the energy savings for mechanical pulping by fungal pretreatment of both aspen
and loblolly pine chips.
Fungal species and wood effects. We compared the energy requirement for mechanical
pulping of chips treated for four weeks with fungi in either stationary or rotating bioreactors. The
efficacy of the individual fungal treatments were dependent on the type of wood tested. The
percentage of energy saved in producing 100-ml Canadian standard freeness (CSF) pulp ranged
from insignificant for aspen treated with
to as much as 47% far aspen treated
with Phlebia brevispora and 68% for loblolly pine treated with
(Fig. 1). Substantial energy savings were also obtained for aspen treated with
(35%) and loblolly pine treated with
Chip movement effects. Comparisons of two fungi on aspen chips in both rotating drums
and stationary trays showed that fungal pretreatment was sensitive to chip movement. With
movement, energy savings increased 3.8-fold (to 38%) with
2.7-fold (to 7%) with
Energy-saving stage. Comparison of the patterns for energy consumption dining pulping of
fungal-treated chips (Fig. 1) with that of nontreated chips showed that the treatments facilitated
wood fiber separation (Fig. 2). The bulk of the energy savings occurred early in pulping when
the chips were fiberized into the first coarse pulp (300- to 700-ml CSF). After fiberization, the
energy required to refine the pulps to a given CSF was similar for untreated and treated chips
(nearly parallel refining lines for the different fungal treatments; Fig. 2). The only exception was
the treatment of loblolly pine with C. subvermispora, which gave significant energy savings both
during fiberization and subsequent refining (Fig. 2). The energy consumption patterns indicate
that the coarser the pulp used in papermaking, the more energy saved.
Relationship of chip degradation to energy savings. To determine the basis for energy
savings, we investigated the effects of the fungal treatments shown in Fig. 1 on both chip weight
loss and Klason lignin loss (Fig. 3). Little degradation of either aspen or loblolly pine chips was
required for maximal energy savings. Treatments resulting in minimal chip weight loss (< 5%)
were capable of giving substantial energy savings. Over the range of fungi and treatment
conditions tested, no definitive correlations occurred between the extent of energy savings and
either bulk weight or Klason lignin loss. Treatment of loblolly pine chips typically resulted in
energy savings equivalent to those obtained with aspen, but at much lower lignin loss. Although
treatment efficacy is apparently not due to bulk lignin loss, we cannot rule out limited lignin
modification, such as a decrease in the degree of lignin polymerization, or lignin degradation in a
limited specific zone.
Relationship of paper Strength to energy savings. Using handsheets produced from chips
treated with the test fungi, we investigated whether or not fungal treatments that resulted in energy
savings also resulted in increased sheet strength. Certain fungal treatments of aspen, including
P. tremellosa in a stationary wire tray and P. chrysosporium in a rotating drum, resulted in high
relative energy savings as well as high relative burst, tensile, and tear indexes ( e.g., burst index
shown in Fig. 4). However, over the range of fungi and conditions tested for aspen, the extent of
energy savings for a given treatment did not correlate with the level of improvement for burst,
tensile, and tear indexes ( e.g., burst index shown in Fig. 4). For loblolly pine, substantial energy
savings occurred with no significant change in strength ( e.g., burst index shown in Fig. 4).
that certain high-yield fungal treatments of both aspen and loblolly
in substantial energy
Most energy is
saved during chip fiberization.
Fungal species, wood type, and chip movement during treatment
can all markedly affect the amount of energy saved.
strength improvements nor energy
savings depended on bulk loss of chip weight or Klason lignin content. Treatments resulting in
the highest energy savings did not necessarily result in the highest strength properties. Certain
fast-growingfungal Species within the genera
the most promise for further research.
Further research is required to (1) determine the chemical-physical and biochemical basis for
energy savings and strength increase in both hardwoods and softwoods, (2) apply this knowledge
in developing more efficient screening methods, and (3) use these methods to optimize both
energy savings and strength properties for a given fungal treatment.
Fungi, chip medium. bioreactors. and treatment conditions. The following white-rot fungi,
maintained on potato dextrose agar (Difco Laboratories, Detroit, MI.) slants, were used (#
(Karst.) Reid #TON-427,
) #BKM-F-1767 (BKM),
Galz.) Donk #RLG-6074,
Phlebia (Merulius) tremellosa
(Schaeff.:Fr.) Kumm. #OKM-2994, and
(L.:Fr.) Pilát #MAD-697. The fresh, standard,
industrial-type 19-mm white aspen (
Michx.) chips used for inoculum and treatments,
nutrient supplements (minus glucuronic and salicylic acids), inoculation method, aeration with
humidified air, and drum rotation schedule (1 rev·h-1
; initial rotation schedule as for
were described previously (16). The bioreactors consisted of rotating
stainless-steel nonperforated drum bioreactors, otherwise identical to the perforated drum
bioreactors described previously (16), or stationary stainless-steel stationary wire trays (570 by
480 by 60 mm) placed within sterile autoclavable polypropylene bags. All fungi were incubated
1°C except for
which was incubated at 39
Refining energy measurements. Energy was measured by fiberizing chips and refining
pulps (approximately 1 to 5 kg ovendry weight) over a 30- to 250-sinterval in a Sprout-Waldron
model D 2202 *single, rotating, 305-mm-diameter disk mechanical refiner operated at
atmospheric pressure. The energy consumed was measured using an Ohio Semitronics, Inc.
model WH 30-11195 integrating watt meter that was attached to the power supply side of the
driving 44.8 kW electric motor. Automated data acquisition was performed by an AT&T PC
6300 computer using Lotus Measure (Lotus Corp.). Values for pulping and refining energy are
reported as kW·h·kg-1
(ovendry) with the idling (without chip or pulp load) energy subtracted.
* The use of trade of firm names in this publication is for reader information and use does not imply endorsement by the U.S. Department of Agriculture of any product or service.